Presentation on theme: "Global and Turkish Perspectives of Thorium Fuel for Nuclear Energy Prof. Dr. Muammer Kaya Osmangazi University Mining Engineering Department, Eskişehir-Turkey."— Presentation transcript:
Global and Turkish Perspectives of Thorium Fuel for Nuclear Energy Prof. Dr. Muammer Kaya Osmangazi University Mining Engineering Department, Eskişehir-Turkey
Natural Properties of Thorium (Th) (Earth’s Forgotten Treasure) Occurs naturally, Identified almost two centuries ago, Exists in nature almost entirely as stable Th-232 isotope, Th itself cannot sustain a nuclear chain reaction, Is a lustrous silvery-white metal, Is dense and only slightly radioactive actinides, you can carry a lump of it in your pocket without harm (less radiotoxic), Th is fertile material, accept a neutron and transmute into fissile U-233 and decays to stable Pb-208. Th is usually a by-product of the REE containg monazite or bastnasite minerals.
THORIUM BASICS (New Green Nuke Nuclear Renaissance) Is plentiful in nature and virtually inexhaustable fuel. Is a thermal breeder (i.e. creates enough new fuel as it breaks down to sustain a high-temperature chain reaction indefinitely). It is impossible to make nuclear weapons and/or bombs from Th by terrorists (i.e. peaceful) Nuclear power without proliferation has obvious political appeal for governments. Has a high heat capacity (i.e. smaller reactors) Does not require costly mining and mineral processing methods (i.e. less expensive), Is extraordinally efficient nuclear fuel (i.e. allows longer fuel burn-up) Produces more neutrons per collision; thus 20-40 times more energy is generated, less fuel consumed and 47 times less radioactive nasties left behind. Th fuel is completely used up in the reactor; thus, there is relatively little nuclear waste. Th waste needs to be stored for only few hundred years (as long as 300 years) not for a few thousand (10000 years) like U wastes. Th reactors has zero risk of melt down as opposed to U reactors. Th reactors can use liquid fuel which has significant advantages in operation, control and processing over solid fuels. Liquid fuels works at high temperature without pressurization. “Th should be heart of the nations’ atomic power effort”
WHY Thorium ? (New Era of Safe, Clean and Affordable Energy) There is a treat of climate change, There is an urgent demand for carbon-free energy/electricity. Th is 3-4 times more abundant than U in nature and distrubuted evenly in most countries in the world. Th can be mined with relatively low-cost and environment friendly mining methods from high grade alluvial deposits. Th extraction is relatively straightforward. Th has a better radiation stability and longer fuel cycle. Th has a higher energy density and fuel economy. Th wastes have a less radiotoxic period due to absence of transuranic wastes (i.e. Pu, Np, Ce and Am). Th mixed oxide (TMOX (Pu+Th)) fuel can be burned in any reactor that is lisenced to use MOX. There is a huge spent toxic material/plutonium that has being piled up from U- fuel. Th fuel can be used to safely incinerate these unwanted stockpiles. Global energy needs for one year can be supplied by approximately 6600 tons of Th.
URANIUM (Today’s problematic nuclear fuel) Today’s prefered fuel in commercial reactors, U has been adequate to meet today’s supply needs, Reserve: 5.5*10 6 tons; Yearly Production: 65*10 3 tons, Producers: 19; Life Expectancy: 50-60 years U ores are generally not harmful, but is dangerously toxic to humans if ingested, inhaled or even of prolonged contact. Reactors requires exteremely rare 235 U (0.7%) which must be purified/ enriched from natural 238 U. U mining, enrichment and extraction are expensive and complex, U-fuel leaves large amount of toxic wastes containing Pu-239 that can be used in making bombs and weapons, The used/depleted fuel can be reprocessed by expensive Pu-U extraction (Purex) process to remove fissile material and refabricate new fuel elements, R&D on U will fade away in favour of Th.
CountryRAR Th (tonnes) EAR Th (tonnes) Brazil606,000700,000 Turkey380,000500,000 India319,000- United States137,000295,000 Norway132,000 Greenland54,00032,000 Canada45,000128,000 Australia19,000- South Africa18,000- Egypt15,000309,000 Other Countries 505,000- World Total2,230,0002,130,000 Reasonably Assured Reserves (RAR) and Estimated Additional Reserves (EAR) of thorium by OECD/NEA, Nuclear Energy, "Trends in Nuclear Fuel Cycle", Paris, France (2001). (http://en.wikipedia.org/wiki/Thorium)
MONAZITE (REE-Th PO 4 ) A phosphate mineral with Rare Earth Oxide (REO) content of 70% (Ce, La, Pr and Nd). Monazite is found in granites, syanites, pegmatites, beach sands etc. World monazite resources are estimated to be about 12 million tons. Includes 3-14% Th and variable amount of U. Found in placer deposites, beach sands and is also a component of the Bayan Obo deposit in China. World monazite production is between 5000-6000 tons/y. Major Monazite producers are Mt Weld (Australia), (Andhra Pradesh, Tamil Nuda, Odisha) India and Guandong (China), Malaysia and Brazil.
ThO 2 Mining from Monazite Th from monazite deposits can be mined with realtively low-cost and environment friendly mining methods, because it exists in high concentrations and in high-grades at the surface or in beach sands. The ore/sand can be skimmed off the surface by dredge mining. Monazite mining is more economical due to presence of Th as a by- product in the REE ore. U mine can be developed in 10-15 years, Th mine can be developed in 2-3 years due to less requlatory scrutiny. ThO 2 is liberated from monazite by gravitational, magnetic and electrostatic concentration methods, employing a minimum of dangerous chemicals (i.e. acids). Whereas U is mined by expensive underground mining and in-situ acid leaching methods.
BASTNASITE (REE-ThFCO 3 2 ) A fluorocarbonate mineral with a REO content of approximately 70% (Ce, La, Pr and Nd). Basnasite is the primary source of ligth REOs and accounts for 80% of the overall amount of REO in the world. In the last 50 years basnasite replaced monazite as a chief mineral source of REEs. Basnasite has been extracted on a large scale only in Mountain Pass, USA and Bayan Obo, China (supply 45% of world demand). Expensive underground mining methods are used. Processing depends on fine grinding; gravity, magnetic and flotation separations; calcination, HCl leaching and solvent extraction steps.
Uranium and Thorium Deposits of Turkey Black Sea Mediterranean Sea Ankara Eskisehir Sivrihisar-Eskisehir Ligth REE+Th Deposit
Typical TREO content Kaynak: Greenfields Research Ltd; (Data: Company websites) 1 st Quartile Comparison of some REO Deposits according to Reserve Size 13 11.
Kaynak: Greenfields Research Ltd; Data: Company websites ThO 2 contents of some REO Deposits 14 3.
Reserve Development Studies in Eskişehir- Sivrihisar-Kızılcaören Light REEs+Th Field First reserve calculations depended on 50-200 m deep drilling studies in 1959. In 2011, two 500 m deep drilling bores were opened. Analyses showed further reserves at deeps. In 2012; 10,000 m drilling were performed at 38 locations. Between 2014 and 2017; 116,000 m drilling will be performed at 289 locations. 45,000 samples will be taken for geochemical and 1,000 samples will be taken by XRD analyses. First reserve calculations depended on 50-200 m deep drilling studies in 1959. In 2011, two 500 m deep drilling bores were opened. Analyses showed further reserves at deeps. In 2012; 10,000 m drilling were performed at 38 locations. Between 2014 and 2017; 116,000 m drilling will be performed at 289 locations. 45,000 samples will be taken for geochemical and 1,000 samples will be taken by XRD analyses. 15 Exploration with drilling Drilling cores
Eti Mines Eskişehir-Sivrihisar Deposit’s Operation Plan Mineral: Bastnasite Ore Charecteristic: Complex, finely disseminated, Ores: Layers, lenses and veins besides impregnation and brecciated zones (Hydrothermal deposit). Area: 1,758 hectare Reserve: 30,358,268 ton Mineral Grade Distribution: 37.44 % CaF 2, 31.04 % BaSO 4 and 3.14 % REE (Ce (2.01%)+La (1.5%)+ Nd (0.39)) 0.21% ThO 2 Along with psilomelan, ilmenite, rutil and some mica minerals. Proved + Probable Mineral Reserve (1977) Distribution (ton) Florite: 11,366,135 tons Barite : 9,424,424 tons REE: 953,587 tons (CeO 2 +La 2 O 3 +Nd 2 O 3 ) Thorium: 380,000 tons Gangue: 8,612,182 tons. Eti Mine prepared a feasibility report for; 10,000 ton/y REO 72,000 ton/y Barite 70,000 ton/y Florite 250 ton/y Thorium production. Mining: Open pit mining will be carried out by Eti Mines of Turkey Mineral Processing/Enrichment: Performed by Domestic and/or Foreign private expert company with service procurement tender for 10 years. Products: Marketed by Eti Mines. ThO 2 will be stored. 16 Operating license owned by Turkish Government Mining Company of Eti Mines for 10 years Deposit discovered using air prospecting survey by General Directorate of Mineral Research and Exploration of Turkey (MTA) in 1959. Ore PropertiesProduction Plan
MONOZITE CRACKING/OPENING WITH HOT CONCENTRATED H 2 SO 4 Th has been extracted from monazite through a complex multi-stage process (AMEX). Monazite is dissolved in 120-150 o C hot concentrated H 2 SO 4 for several hours. Th is extracted as an insoluable residue into an organic phase containg an alkyl amine. Then it is separated/ stripped using an ion such as nitrate, chloride, hydroxide or carbonate returning Th to an aqueous phase. Finally Th is precipiteted and collected. Th extraction is a complex process because of similar chemical properties with REOs. Ammonium oxalate Th+REOs RE oxalates Filtering
THORIUM CONCENTRATION FLOWSHEET ORE HNO 3 or H 2 SO 4 LEACHING (pH:1.2) Precipitation of some impurities Solvent Extraction (SX) or Ion Exchange (IE) Th(NO 3 ) 4.nH 2 O Drying (105 o C, 20h) Water Th(NO 3 ) 4 Calcination (575 o C) ThO 2 concentrate ION EXCHANGE RESINE BEADS
EFFECTS OF ROASTING and THIOUREA ADDITION on BASTNASITE LEACHING (Yörükoğulları, Obut, Girgin, 2002 and 2003) 1. Pre-concentration Scrubbing (75% solids, N: 2060 rpm, t: 15 min.) BaSO 4 FlotationPre-Concentrate (21.3% REO) CaF 2 Flotation 2. Bastnasite Pre-Concentrate Leach Particle Size: 0.053 mm N: 450 rpm REEs in solution were analysed by ICP spectrometer. Ba and high S/L: 1/20 g/mL t: 6 hours concentration REE were anaysed by gravimetric methods based on sulphate and oxalate precipitation. 2a. Leaching without Roasting using Concentrated Acids 8M HNO 3 70 o C 100% total REE dissolution 15 M H 2 SO 4 25 o C 89.25% 2.5M HCl 55 o C 82.2% 2b. Roasting+Dilute Acid Leaching After roasting at 750 o C for 1 h, leaching with 1-3M H 2 SO 4 at 25 o C. (Roasting decomposes carbonates and oxidize Ce). Total REE contents for unroasted: 18.59%, roasted: 22.00% and roasted+leached 47.4%. 2c. Roasting+Dilute Acid Leaching and Thiourea Addition (extracting agent for Au, Ag and REE) Thiourea conc.: 0-2 M and 1-3 M H 2 SO 4 Roasted without thiourea: 17.6% REE dissolution Roasted with thiourea: 89.0% dissolution (at 3M H 2 SO 4 and 1M thiourea) 3. Hydroxide-Oxalate Mixture Precipitation (Mish metal) from Leach Solution+ Heating to 900 o C for 2 hours Total REE 93.6%, REO: 92.6%
EFFECTS OF ROASTING and THIOUREA ADDITION on BASTNASITE LEACHING (Yörükoğulları, Obut, Girgin, 2002 and 2003) Roasting decomposes the flurocarbonate structure of REEs in the preconcentrate with the formation of fluocerite and cerianite as new phases (XRD results). This change in composition increases the selective dissolution of lanthanum and neodymium in H 2 SO 4 solution causing 5.6 times increase in the total REs dissolution. Addition of thiourea (CS(NH 2 ) 2 ) to the leaching medium increases the dissolution of total REEs in the unroasted and especially in the roasted pre concentrate reaching a dissolution of 89%. 92.6% mixed REO precipitation with H 2 SO 4 -thiourea medium was achived.
PİLOT SCALE ACID LEACH and SOLVENT EXTRACTION TESTS for REEs and Th from ESKISEHIR ORE by MTA (2004) Particle size: - 1mm; Oxidizing Roasting Temperature: 600-900 o C; t: 1-6 hours Leach: 3 M H 2 SO 4 REE dissolution: 86% (Ce, La, Nd ve Th) and 3 M HCl REE dissolution: 92% (Ce, La, Nd ve Th) (89% REO mishmetal) Oxalate Precipitation: Th Grade: 98.7%, Th Recovery: 98% Blending Jaw Crusher Cone Crusher Roll Crusher Rotating Furnace Oxidizing Roasting 3M HCl acid leach Filtration Cake Filtrate Solution FlotationOxalate precipitation REOs+ThO 2 Run-of-mine ores from 3 districts 93% BaSO 4 84% CaF 2 98.7% Th(N0 3 ) 4 84.2% Ln(OH) 3 84%CeO 2
The Effects of Particle Size and Roasting Time on Thorium Recovery during H 2 SO 4 and HCl Leaching (Yorukoglu et.al., 2012) Sample: 3 t representative homogenized Particle Sizes Tested: 0.065, 0.2, 1 and 3 mm Oxidizing Roasting Temp. and Time: 900 o C and 1, 3 and 6 hours Leaching: 3 M H 2 SO 4 and 3 M HCl, 3 h, 25 o C, separately Leaching Recovery: (REEs + Th) % R = 79%, 1 mm, 1h R = 73%, 1 mm, 3 h 3 M H 2 SO 4 3 M HCl
The Effects of Particle Size and Roasting Time on Thorium Recovery during H 2 SO 4 and HCl Leaching (Yorukoglu et.al., 2012) 3 M H 2 SO 4 gives better leaching recovery than HCl. H 2 SO 4 is cheaper than HCl. Oxidizing roasting at 900 o C at 1 hour, before athmosferic leaching is necessary. The best particle size for leaching is 1 mm. 79% (REEs+Th) dissolution can be achieved.
CONCLUSIONS from TURKEY’S POINT OF VIEW Energy is major concern for developing Turkish society. Turkey today exports more than 70% of its energy as fossil fuels. In the last 50 years, Turks are sceptical, anxious and indecisive about having nuclear energy. In the last 10 years, we are bringing Th into Turkish government’s attention and national discussion as a new, safe, clean, affortable, CO 2 -free, alterternative, strategic and domestic nuclear energy fuel. In Turkey, we are trying to find funds to support education and R&D on Th. We are expecting to establish Thorium Research Center /ThoReC) in Turkey for Th mining+enrichment+extraction+fuel fabrication+prototype reactor testing+nuclear fuel cycle testing. Turkey recently contacted four VVER-1200 type Russian Nuclear Power Reactors using U as a fuel in Akkuyu (Rosatom) and another four units will be established in Sinop in the next decade by Japan (Mitsubishi- Westinghouse). We will enforce government to use Th along with U as an alternative fuel in the new reactors. If Turkey can process it’s important domestic low grade bastnasite resource in Eskisehir for Th, it can suppy its own Th fuel for more than 100 years and become self-sufficient in energy sources.
THANKS FOR YOUR INTEREST
Comparing Reactors U Fueled Light Water Reactor U+Th Seed and Blanket Reactor Th Liquid Fluoride Reactor FuelU fuel rodsTh+U oxide rodsTh+U fluoride solution Fuel input per GW output * 250 tons raw U2.4 tons raw Th + 177 tons raw U 1 ton raw Th Annual fuel cost for 1 GW reactor $50-60 million $10000 CoolantWater Self requlating (FLiNaK) salt/gas Proliferation potential MediumNone Footprint200000-300000 ft 2 surrounded by a low-density population zone 2000-3000 ft 2 With no need for a buffer zone. Richard Martin (2009) * equvalent energy from 3.5 million tons of coal
D ü nya enerji ihtiyacını toryum tek başına 6600 ton ile karşılayabilecektir.
MINERALGRAIN SIZE (micron)CONTENT (%) Fluorite2-400038-45 Barite10-140019-36 Bastnasite7-26 Opak Minerals12-120020-22 REE and Th are in fine size fraction
HCl Leaching of Sivrihisar Bastnasite Ore (Gülmez et.al., 2012) Sample: 3 t representative homogenized Particle Sizes Tested: 0.065, 0.2, 1 and 3 mm Leaching: 3 M H 2 SO 4 and HCl, 3 h, 25 o C, separately Leaching Recovery: 92.09 % ( REE + Th) Mishmetal concentrate: 73.8% REE/89.4%REO (saleable) FBaOCeO2La2O3Nd2O3ThO2SO3Ca 20.80 2.011.50.40.112.120.3 FBaOCeO2La2O3Nd2O3ThO2SO3Fe2O3 25.1022.300.500.400.100.01313.63.60 HCl Leaching Tailing Chemical Analyses Chemical Analyses of Composite Sample
Comparison of some REO Deposits according to REO Grades 30
MONAZITE ALKALINE CRACKING and AUTOCLAVING WITH NaOH Hot 73% NaOH solution is used to crack/open monazite sand. After addition of cold water Na-phosphate is removed from the solution. REO and Th(OH) 4 in solid residue were leached with HCl (pH: 3-4). Dewatered mishmetal RE chlorides are produced with electrolitic reduction. Using liquid-liquid extraction with Chelating reagents can give 99.99% pure products. Th recovery from monazite usually involves leaching with NaOH at 140 o C followed by complex processes to precipitate pure ThO 2
THORIUM CONCENTRATION STUDIES BEDRI IPEKOGLU (Ph.D Thesis, 1983) SİVRİHİSAR-ESKISEHIR ORE GRAVITY CONCENTRATION MAGNETIC CONCENTRATION FLOTATION ACID LEACHING Optimum Conditions: HCl dosage: 200kg/t Leaching Time: 3 hours Th Grade: %99 ACID TOREX PROCESS ThO 2 recovery from used (U 233 /Th) fuel Hot acid leach (13M HNO 3, 0.05M HF, 0.1M Al nitrat at boiling temperature) Centrifuging Solid residue Th(NO 3 ) 4 + UO 2 (NO 3 ) 2 Solution SX Columns Purification Tributyl phosphate (TBP)